Polymer degradation

Short description: Alteration in the polymer properties under the influence of environmental factors

Template:TopicTOC-Polymer

Polymer degradation is the lowering of a polymer, such as strength, caused by changes in its chemical composition. Polymers and particularly plastics are subject to degradation at all stages of their product life cycle, including during their initial processing, use, disposal into the environment and recycling.[1] The rate of this degradation varies significantly; biodegradation can take decades, whereas some industrial processes can completely decompose a polymer in hours.

Technologies have been developed to both inhibit or promote degradation. For instance, polymer stabilizers ensure plastic items are produced with the desired properties, extend their useful lifespans, and facilitate their recycling. Conversely, biodegradable additives accelerate the degradation of plastic waste by improving its biodegradability. Some forms of plastic recycling can involve the complete degradation of a polymer back into monomers or other chemicals.

In general, the effects of heat, light, air and water are the most significant factors in the degradation of plastic polymers. The major chemical changes are oxidation and chain scission, leading to a reduction in the molecular weight and degree of polymerization of the polymer. These changes affect physical properties like strength, malleability, melt flow index, appearance and colour. The changes in properties are often termed "aging".

2013 European plastic demand by polymer type:
PP: polypropylene, PE: polyethylene, PVC: Polyvinyl chloride, PS: Polystyrene, PET: Polyethylene terephthalate

## Contents

* 1 Susceptibility
* 2 Degradation during processing
* 2.1 Thermal oxidation
* 2.2 Thermal degradation
* 2.3 Thermo-mechanical degradation
* 3 In-service degradation
* 3.1 Chlorine-induced cracking
* 3.2 Electronics
* 3.3 Galvanic action
* 4 Degradation in the environment
* 4.1 Photo-oxidation
* 4.2 Hydrolysis
* 4.3 Ozonolysis of rubbers
* 4.4 Biological degradation
* 5 Degradation during recycling
* 5.1 Remelting
* 5.2 Thermal depolymerisation & pyrolysis
* 5.3 Chemical depolymerisation
* 6 Stabilisers
* 7 Detection
* 8 See also
* 9 Bibliography
* 10 References

## Susceptibility

Plastics exist in huge variety, however several types of commodity polymer dominate global production: polyethylene (PE), polypropylene (PP), polyvinyl chloride (PVC), polyethylene terephthalate (PET, PETE), polystyrene (PS), polycarbonate (PC), and poly(methyl methacrylate) (PMMA). The degradation of these materials is of primary importance as they account for most plastic waste.

These plastics are all thermoplastics and are more susceptible to degradation than equivalent thermosets, as those are more thoroughly cross-linked. The majority (PP, PE, PVC, PS and PMMA) are addition polymers with all-carbon backbones that are more resistant to most types of degradation. PET and PC are condensation polymers which contain carbonyl groups more susceptible to hydrolysis and UV-attack.

## Degradation during processing

Plastic compounding scheme

File:Plastic Injection Molding.webm

Thermoplastic polymers (be they virgin or recycled) must be heated until molten to be formed into their final shapes, with processing temperatures anywhere between 150-320 °C (300–600 °F) depending on the polymer.[2] Polymers will oxidise under these conditions, but even in the absence of air, these temperatures are sufficient to cause thermal degradation in some materials. The molten polymer also experiences significant shear stress during extrusion and moulding, which is sufficient to snap the polymer chains. Unlike many other forms of degradation, the effects of melt-processing degrades the entire bulk of the polymer, rather than just the surface layers. This degradation introduces chemical weak points into the polymer, particularly in the form of hydroperoxides, which become initiation sites for further degradation during the object's lifetime.

Polymers are often subject to more than one round of melt-processing, which can cumulatively advance degradation. Virgin plastic typically undergoes compounding to introduce additives such as dyes, pigments and stabilisers. Pelletised material prepared in this may also be pre-dried in an oven to remove trace moisture prior to its final melting and moulding into plastic items. Plastic which is recycled by simple re‑melting (mechanical recycling) will usually display more degradation than fresh material and may have poorer properties as a result.[3]

### Thermal oxidation

Although oxygen levels inside processing equipment are usually low, it cannot be fully excluded and thermal-oxidation will usually take place more readily than degradation that is exclusively thermal (i.e. without air).[4] Reactions follow the general autoxidation mechanism, leading to the formation of organic peroxides and carbonyls. The addition of antioxidants may inhibit such processes.

### Thermal degradation

Main article: Chemistry:Thermal degradation of polymers

Heating polymers to a sufficiently high temperature can cause damaging chemical changes, even in the absence of oxygen. This usually starts with chain scission, generating free radicals, which primarily engage in disproportionation and crosslinking. PVC is the most thermally sensitive common polymer, with major degradation occurring from ~250 °C (480 °F) onwards;[5] other polymers degrade at higher temperatures.[6]

### Thermo-mechanical degradation

Molten polymers are non-Newtonian fluids with high viscosities, and the interaction between their thermal and mechanical degradation can be complex. At low temperatures, the polymer-melt is more viscous and more prone to mechanical degradation via shear stress. At higher temperatures, the viscosity is reduced, but thermal degradation is increased. Friction at points of high sheer can also cause localised heating, leading to additional thermal degradation.

Mechanical degradation can be reduced by the addition of lubricants, also referred to as processing aids or flow aids. These can reduce friction against the processing machinery but also between polymer chains, resulting in a decrease in melt-viscosity. Common agents are high-molecular-weight waxes (paraffin wax, wax esters, etc.) or metal stearates (i.e.zinc stearate).

## In-service degradation

Global plastic waste generation by industrial sector for 2015, measured in tonnes per year

Most plastic items, like packaging materials, are used briefly and only once. These rarely experience polymer degradation during their service-lives. Other items experience only gradual degradation from the natural environment. Some plastic items, however, can experience long service-lives in aggressive environments, particularly those where they are subject to prolonged heat or chemical attack. Polymer degradation can be significant in these cases and, in practice, is often only held back by the use of advanced polymer stabilizers. Degradation arising from the effects of heat, light, air and water is the most common, but other means of degradation exist.

The in-service degradation of mechanical properties is an important aspect which limits the applications of these materials. Polymer degradation caused by in-service degradation can cause life threatening accidents. In 1996, a baby was fed via a Hickman line and suffered an infection, when new connectors were used by a hospital. The reason behind this infection was the cracking and erosion of the pipes from the inner side due to contact with liquid media.[7]

### Chlorine-induced cracking

Chlorine attack on an acetal resin plumbing joint

Drinking water which has been chlorinated to kill microbes may contain trace levels of chlorine. The World Health Organization recommends an upper limit of 5 ppm.[8] Although low, 5 ppm is enough to slowly attack certain types of plastic, particularly when the water is heated, as it is for washing. Polyethylene,[9][10] polybutylene [11] and acetal resin (polyoxymethylene)[12] pipework and fittings are all susceptible. Attack leads to hardening of pipework, which can leave it brittle and more susceptible to mechanical failure.

### Electronics

Plastics are used extensively in the manufacture of electrical items, such as circuit boards and electrical cables. These applications can be harsh, exposing the plastic to a mixture of thermal, chemical and electrochemical attack. Many electric items like transformers, microprocessors or high-voltage cables operate at elevated temperatures for years, or even decades, resulting in low-level but continuous thermal oxidation. This can be exacerbated by direct contact with metals, which can promote the formation of free-radicals, for instance, by the action of Fenton reactions on hydroperoxides.[13] High voltage loads can also damage insulating materials such as dielectrics, which degrade via electrical treeing caused by prolonged electrical field stress.[14][15]

### Galvanic action

Mechanism of galvanic degradation of high temperature polyimide thermoset polymer

Polymer degradation by galvanic action was first described in the technical literature in 1990 by Michael C. Faudree, an employee at General Dynamics, Fort Worth Division.[16][17] The phenomenon has been referred to as the "Faudree Effect",[18] and can possibly be used as a sustainable process to degrade non-recyclable thermoset plastics, and also has had implications for preventing corrosion on aircraft for safety such as changes in design.[19][20] When carbon-fiber-reinforced polymer is attached to a metal surface, the carbon fiber can act as a cathode if exposed to water or sufficient humidity, resulting in galvanic corrosion. This has been seen in engineering when carbon-fiber polymers have been used to reinforce weakened steel structures.[21][22] Reactions have also been seen in aluminium[23] and magnesium alloys,[24] polymers affected include bismaleimides (BMI), and polyimides. The mechanism of degradation is believed to involve the electrochemical generation of hydroxide ions, which then cleave the amide bonds.[25]

## Degradation in the environment

Most plastics do not biodegrade readily,[26] however, they do still degrade in the environment because of the effects of UV-light, oxygen, water and pollutants. This combination is often generalised as polymer weathering.[27] Chain breaking by weathering causes increasing embrittlement of plastic items, which eventually causes them to break apart. Fragmentation then continues until eventually microplastics are formed. As the particle sizes get smaller, so their combined surface area increases. This facilitates the leaching of additives out of plastic and into the environment. Many controversies associated with plastics actually relate to these additives.[28][29]

### Photo-oxidation

Main article: Chemistry:Photo-oxidation of polymers

Photo-oxidation is the combined action of UV-light and oxygen and is the most significant factor in the weathering of plastics.[27] Although many polymers do not absorb UV-light, they often contain impurities like hydroperoxide and carbonyl groups introduced during thermal processing, which do. These act as photoinitiators to give complex free radical chain reactions where the mechanisms of autoxidation and photodegradation combine. Photo-oxidation can be held back by light stabilizers such as hindered amine light stabilizers (HALS).[30]

### Hydrolysis

Polymers with an all-carbon backbone, such as polyolefins, are usually resistant to hydrolysis. Condensation polymers like polyesters,[31] polyamides, polyurethanes and polycarbonates can be degraded by hydrolysis of their carbonyl groups, to give lower molecular weight molecules. Such reactions are exceedingly slow at ambient temperatures, however, they remain a significant source of degradation for these materials, particularly in the marine environment.[32] Swelling caused by the absorption of minute amounts of water can also cause environmental stress cracking, which accelerates degradation.

### Ozonolysis of rubbers

Main articles: Chemistry:Ozonolysis and Ozone cracking

Ozone cracking in natural rubber tubing

Polymers, which are not fully saturated, are vulnerable to attack by ozone. This gas exists naturally in the atmosphere but is also formed by nitrogen oxides released in vehicle exhaust pollution. Many common elastomers (rubbers) are affected, with natural rubber, polybutadiene, styrene-butadiene rubber and NBR being most sensitive to degradation. The ozonolysis reaction results in immediate chain scission. Ozone cracks in products under tension are always oriented at right angles to the strain axis, so will form around the circumference in a rubber tube bent over. Such cracks are dangerous when they occur in fuel pipes because the cracks will grow from the outside exposed surfaces into the bore of the pipe, and fuel leakage and fire may follow. The problem of ozone cracking can be prevented by adding antiozonants.

### Biological degradation

Main articles: Chemistry:Synthetic biodegradable polymer, Biodegradable plastic, Biodegradable polymer, and Plastic degradation by marine bacteria

The major appeal of biodegradation is that, in theory, the polymer will be consumed in the environment without needing complex waste management and that the products of this will be non-toxic. Most common plastics biodegrade very slowly, sometimes to the extent that they are considered non-biodegradable.[26][33] As polymers are ordinarily too large to be absorbed by cells, biodegradation initially relies on secreted extracellular enzymes to lower the chain-lengths. This requires the polymers bear functional groups the enzymes can 'recognise', such as ester or amide groups. Long-chain polymers with all-carbon backbones like polyolefins, polystyrene, and PVC will not degrade by biological action alone.[34] and They must first be oxidised to create chemical groups which the enzymes can attack.[35][36]

Oxidation can be caused by melt-processing or weathering. Oxidation may be intentionally accelerated by the addition of biodegradable additives. These are added to the polymer during compounding to improve the biodegradation of otherwise very resistant plastics. Similarly, biodegradable plastics have been designed which are intrinsically biodegradable, provided they are treated like compost and not just left in a landfill site where degradation is very difficult because of the lack of oxygen and moisture.[37]

## Degradation during recycling

Main article: Physics:Plastic recycling

Global means of disposal for plastic waste

The act of recycling plastic degrades its polymer chains, usually as a result of thermal damage similar to that seen during initial processing. In some cases, this is turned into an advantage by intentionally and completely depolymerising the plastic back into its starting monomers, which can then be used to generate fresh, un-degraded plastic. In theory, this chemical (or feedstock) recycling offers infinite recyclability, but it is also more expensive and can have a higher carbon footprint because of its energy costs.[3] Mechanical recycling, where the plastic is simply remelted and reformed, is more common, although this usually results in a lower-quality product. Alternatively, plastic may simply be burnt as a fuel in a waste-to-energy process.[38][39]

### Remelting

Thermoplastic polymers like polyolefins can be remelted and reformed into new items. This approach is referred to as mechanical recycling and is usually the simplest and most economical form of recovery.[3] Post-consumer plastic will usually already bear a degree of degradation. Another round of melt-processing will exacerbate this, with the result being that mechanically recycled plastic will usually have poorer mechanical properties than virgin plastic.[40] Degradation can be enhanced by high concentrations of hydroperoxides, cross-contamination between different types of plastic and by additives present within the plastic. Technologies developed to enhance the biodegradation of plastic can also conflict with its recycling, with oxo-biodegradable additives, consisting of metallic salts of iron, magnesium, nickel, and cobalt, increasing the rate of thermal degradation.[41][42] Depending on the polymer in question, an amount of virgin material may be added to maintain the quality of the product.[43]

### Thermal depolymerisation & pyrolysis

Main article: Chemistry:Thermal depolymerization

As polymers approach their ceiling temperature, thermal degradation gives way to complete decomposition. Certain polymers like PTFE, polystyrene and PMMA[44] undergo depolymerization to give their starting monomers, whereas others like polyethylene undergo pyrolysis, with random chain scission giving a mixture of volatile products. Where monomers are obtained, they can be converted back into new plastic (chemical or feedstock recycling),[45][46][47] whereas pyrolysis products are used as a type of synthetic fuel (energy recycling).[48] In practice, even very efficient depolymerisation to monomers tends to see some competitive pyrolysis. Thermoset polymers may also be converted in this way, for instance, in tyre recycling.

### Chemical depolymerisation

Condensation polymers baring cleavable groups such as esters and amides can also be completely depolymerised by hydrolysis or solvolysis. This can be a purely chemical process but may also be promoted by enzymes.[49] Such technologies are less well developed than those of thermal depolymerisation, but have the potential for lower energy costs. Thus far, polyethylene terephthalate has been the most heavily studied polymer.[50] Alternatively, waste plastic may be converted into other valuable chemicals (not necessarily monomers) by microbial action.[51][52]

## Stabilisers

Main article: Chemistry:Polymer stabilizers

Hindered amine light stabilizers (HALS) stabilise against weathering by scavenging free radicals that are produced by photo-oxidation of the polymer matrix. UV-absorbers stabilise against weathering by absorbing ultraviolet light and converting it into heat. Antioxidants stabilise the polymer by terminating the chain reaction because of the absorption of UV light from sunlight. The chain reaction initiated by photo-oxidation leads to cessation of crosslinking of the polymers and degradation of the property of polymers. Antioxidants are used to protect from thermal degradation.

## Detection

Degradation can be detected before serious cracks are seen in a product using infrared spectroscopy.[53] In particular, peroxy-species and carbonyl groups formed by photo-oxidation have distinct absorption bands.

## See also

* Applied spectroscopy
* Forensic polymer engineering
* Environmental stress fracture
* Polymer engineering
* Weather testing of polymers

## Bibliography

* Lewis, Peter Rhys, Reynolds, K and Gagg, C, Forensic Materials Engineering: Case studies, CRC Press (2004)
* Ezrin, Meyer, Plastics Failure Guide: Cause and Prevention, Hanser-SPE (1996).
* Wright, David C., Environmental Stress Cracking of Plastics RAPRA (2001).
* Lewis, Peter Rhys, and Gagg, C, Forensic Polymer Engineering: Why polymer products fail in service, Woodhead/CRC Press (2010).

## References

1. ↑ Singh, Baljit; Sharma, Nisha (March 2008). "Mechanistic implications of plastic degradation". Polymer Degradation and Stability 93 (3): 561–584. doi:10.1016/j.polymdegradstab.2007.11.008.
2. ↑ Ragaert, Kim; Delva, Laurens; Van Geem, Kevin (November 2017). "Mechanical and chemical recycling of solid plastic waste". Waste Management 69: 24–58. doi:10.1016/j.wasman.2017.07.044. PMID 28823699. Bibcode: 2017WaMan..69...24R.
3. ↑ 3.0 3.1 3.2 Schyns, Zoé O. G.; Shaver, Michael P. (February 2021). "Mechanical Recycling of Packaging Plastics: A Review". Macromolecular Rapid Communications 42 (3). doi:10.1002/marc.202000415. PMID 33000883.
4. ↑ Peterson, Jeffery D.; Vyazovkin, Sergey; Wight, Charles A. (2001). "Kinetics of the Thermal and Thermo-Oxidative Degradation of Polystyrene, Polyethylene and Poly(propylene)". Macromolecular Chemistry and Physics 202 (6): 775–784. doi:10.1002/1521-3935(20010301)202:6<775::AID-MACP775>3.0.CO;2-G.
5. ↑ Yu, Jie; Sun, Lushi; Ma, Chuan; Qiao, Yu; Yao, Hong (February 2016). "Thermal degradation of PVC: A review". Waste Management 48: 300–314. doi:10.1016/j.wasman.2015.11.041. PMID 26687228. Bibcode: 2016WaMan..48..300Y.
6. ↑ Matsuzawa, Yoshiaki; Ayabe, Muneo; Nishino, Junya; Kubota, Nobuhiko; Motegi, Mikio (August 2004). "Evaluation of char fuel ratio in municipal pyrolysis waste". Fuel 83 (11–12): 1675–1687. doi:10.1016/j.fuel.2004.02.006.
7. ↑ Saharudin, Mohd Shahneel; Atif, Rasheed; Shyha, Islam; Inam, Fawad (2015-12-22). "The degradation of mechanical properties in polymer nano-composites exposed to liquid media – a review" (in en). RSC Advances 6 (2): 1076–1089. doi:10.1039/C5RA22620A. ISSN 2046-2069. http://pdfs.semanticscholar.org/55a1/6d743c56b90d87d1aef9c50e25b0ea9ec284.pdf.
8. ↑ Guidelines for drinking-water quality. (Fourth incorporating the first addendum ed.). Geneva: World Health Organization. 2017. ISBN 978-92-4-154995-0.
9. ↑ Hassinen, J (May 2004). "Deterioration of polyethylene pipes exposed to chlorinated water". Polymer Degradation and Stability 84 (2): 261–267. doi:10.1016/j.polymdegradstab.2003.10.019.
10. ↑ Duvall, Donald (June 2014). "Oxidation Resistance of Polypropylene Random Copolymer Pipe to Chlorinated Water". Journal of Failure Analysis and Prevention 14 (3): 336–342. doi:10.1007/s11668-014-9809-3.
11. ↑ Fujii, Takehiro; Matsui, Yuichi; Hirabayashi, Hideo; Igawa, Kazuhisa; Okada, Saori; Honma, Hidekazu; Nishimura, Hiroyuki; Yamada, Kazushi (September 2019). "Influence of residual chlorine and pressure on degradation of polybutylene pipe". Polymer Degradation and Stability 167: 1–9. doi:10.1016/j.polymdegradstab.2019.06.012.
12. ↑ Öner, Mualla; White, Don H. (January 1993). "Investigation of the degradation of commercial polyoxymethylene copolymer in water service applications". Polymer Degradation and Stability 40 (3): 297–303. doi:10.1016/0141-3910(93)90135-6.
13. ↑ Osawa, Zenjiro (January 1988). "Role of metals and metal-deactivators in polymer degradation". Polymer Degradation and Stability 20 (3–4): 203–236. doi:10.1016/0141-3910(88)90070-5.
14. ↑ Zakrevskii, V. A.; Sudar, N. T.; Zaopo, A.; Dubitsky, Yu. A. (15 February 2003). "Mechanism of electrical degradation and breakdown of insulating polymers". Journal of Applied Physics 93 (4): 2135–2139. doi:10.1063/1.1531820. Bibcode: 2003JAP....93.2135Z.
15. ↑ Mayoux, C. (October 2000). "Degradation of insulating materials under electrical stress". IEEE Transactions on Dielectrics and Electrical Insulation 7 (5): 590–601. doi:10.1109/TDEI.2000.879355.
16. ↑ Faudree, Michael C. (1991). "Relationship of Graphite/Polyimide Composites to Galvanic Processes". Society for the Advancement of Material and Process Engineering(SAMPE) Journal 2: 1288–1301. ISBN 0-938994-56-5. http://www.michaelcfaudree.com/2Relationship of Graphite Polyimide Composites to Galvanic Processes.pdf.
17. ↑ C, Faudree M. (1991). "電気化学的過程とグラファイト/ポリイミド複合材料の関係". International Sampe Symposium and Exhibition (Society for the Advancement of Material and Process Engineering) 36 (2): 1288–1301. http://jglobal.jst.go.jp/public/20090422/200902037896192534.
18. ↑ Gnanavel, G.; Thirumarimurugan, M.; Mohana Jeya Valli, V.P (2015). "Current Scenario of Biodegradation of Plastics – Review". Australian Journal of Basic and Applied Sciences 9: 408–417. ISSN 1991-8178. https://www.ajbasweb.com/old/ajbas/2015/July/408-417.pdf.
19. ↑ Dornheim, Michael (November 26, 1990). "ATF Researchers Address Potential for Bismaleimide Composile Degradation". Aviation Week and Science Technology: 122–123. https://archive.aviationweek.com/issue/19901126/.
20. ↑ Faudree, Michael C. (1991). "Relationship of Graphite/Polyimide Composites to Galvanic Processes". Society for the Advancement of Material and Process Engineering(SAMPE) Journal 2: 1288–1301. ISBN 0-938994-56-5. http://www.michaelcfaudree.com/2Relationship of Graphite Polyimide Composites to Galvanic Processes.pdf.
21. ↑ Tavakkolizadeh, Mohammadreza; Saadatmanesh, Hamid (August 2001). "Galvanic Corrosion of Carbon and Steel in Aggressive Environments". Journal of Composites for Construction 5 (3): 200–210. doi:10.1061/(ASCE)1090-0268(2001)5:3(200).
22. ↑ Zhao, Xiao-Ling; Zhang, Lei (August 2007). "State-of-the-art review on FRP strengthened steel structures". Engineering Structures 29 (8): 1808–1823. doi:10.1016/j.engstruct.2006.10.006. Bibcode: 2007EngSt..29.1808Z.
23. ↑ Liu, Z.; Curioni, M.; Jamshidi, P.; Walker, A.; Prengnell, P.; Thompson, G.E.; Skeldon, P. (September 2014). "Electrochemical characteristics of a carbon fibre composite and the associated galvanic effects with aluminium alloys". Applied Surface Science 314: 233–240. doi:10.1016/j.apsusc.2014.06.072. Bibcode: 2014ApSS..314..233L.
24. ↑ Pan, Yingcai; Wu, Guoqing; Cheng, Xu; Zhang, Zongke; Li, Maoyuan; Ji, Sudong; Huang, Zheng (September 2015). "Galvanic corrosion behaviour of carbon fibre reinforced polymer/magnesium alloys coupling". Corrosion Science 98: 672–677. doi:10.1016/j.corsci.2015.06.024. Bibcode: 2015Corro..98..672P.
25. ↑ Woo, E. M.; Chen, J. S.; Carter, C. S. (1993). "Mechanisms of degradation of polymer composites by galvanic reactions between metals and carbon fiber". Polymer Composites 14 (5): 395–401. doi:10.1002/pc.750140505.
26. ↑ 26.0 26.1 Andrady, Anthony L. (February 1994). "Assessment of Environmental Biodegradation of Synthetic Polymers". Journal of Macromolecular Science, Part C: Polymer Reviews 34 (1): 25–76. doi:10.1080/15321799408009632.
27. ↑ 27.0 27.1 Feldman, D. (1 October 2002). "Polymer Weathering: Photo-Oxidation". Journal of Polymers and the Environment 10 (4): 163–173. doi:10.1023/A:1021148205366. Bibcode: 2002JPEnv..10..163F.
28. ↑ Hahladakis, John N.; Velis, Costas A.; Weber, Roland; Iacovidou, Eleni; Purnell, Phil (February 2018). "An overview of chemical additives present in plastics: Migration, release, fate and environmental impact during their use, disposal and recycling". Journal of Hazardous Materials 344: 179–199. doi:10.1016/j.jhazmat.2017.10.014. PMID 29035713. Bibcode: 2018JHzM..344..179H. http://bura.brunel.ac.uk/bitstream/2438/18351/1/FullText.pdf.
29. ↑ Teuten, Emma L.; Saquing, Jovita M.; Knappe, Detlef R. U.; Barlaz, Morton A.; Jonsson, Susanne; Björn, Annika; Rowland, Steven J.; Thompson, Richard C. et al. (27 July 2009). "Transport and release of chemicals from plastics to the environment and to wildlife". Philosophical Transactions of the Royal Society B: Biological Sciences 364 (1526): 2027–2045. doi:10.1098/rstb.2008.0284. PMID 19528054.
30. ↑ Wiles, D.M.; Carlsson, D.J. (November 1980). "Photostabilisation mechanisms in polymers: A review". Polymer Degradation and Stability 3 (1): 61–72. doi:10.1016/0141-3910(80)90008-7. https://nrc-publications.canada.ca/eng/view/accepted/?id=dc80acce-af03-47c8-b44b-f6748a4915a5.
31. ↑ Allen, Norman S.; Edge, Michael; Mohammadian, Mehrdad; Jones, Ken (January 1991). "Hydrolytic degradation of poly(ethylene terephthalate): Importance of chain scission versus crystallinity". European Polymer Journal 27 (12): 1373–1378. doi:10.1016/0014-3057(91)90237-I. Bibcode: 1991EurPJ..27.1373A.
32. ↑ Gewert, Berit; Plassmann, Merle M.; MacLeod, Matthew (2015). "Pathways for degradation of plastic polymers floating in the marine environment". Environmental Science: Processes & Impacts 17 (9): 1513–1521. doi:10.1039/C5EM00207A. PMID 26216708. http://pdfs.semanticscholar.org/1f30/7652fab7d25caf33ff64764d47b594e599a0.pdf.
33. ↑ Ahmed, Temoor; Shahid, Muhammad; Azeem, Farrukh; Rasul, Ijaz; Shah, Asad Ali; Noman, Muhammad; Hameed, Amir; Manzoor, Natasha et al. (March 2018). "Biodegradation of plastics: current scenario and future prospects for environmental safety". Environmental Science and Pollution Research 25 (8): 7287–7298. doi:10.1007/s11356-018-1234-9. PMID 29332271. Bibcode: 2018ESPR...25.7287A.
34. ↑ Danso, Dominik; Chow, Jennifer; Streit, Wolfgang R. (19 July 2019). "Plastics: Environmental and Biotechnological Perspectives on Microbial Degradation". Applied and Environmental Microbiology 85 (19): e01095–19, /aem/85/19/AEM.01095–19.atom. doi:10.1128/AEM.01095-19. PMID 31324632. Bibcode: 2019ApEnM..85E1095D.
35. ↑ Tokiwa, Yutaka; Calabia, Buenaventurada; Ugwu, Charles; Aiba, Seiichi (26 August 2009). "Biodegradability of Plastics". International Journal of Molecular Sciences 10 (9): 3722–3742. doi:10.3390/ijms10093722. PMID 19865515.
36. ↑ Krueger, Martin C.; Harms, Hauke; Schlosser, Dietmar (November 2015). "Prospects for microbiological solutions to environmental pollution with plastics". Applied Microbiology and Biotechnology 99 (21): 8857–8874. doi:10.1007/s00253-015-6879-4. PMID 26318446.
37. ↑ Shah, Aamer Ali; Hasan, Fariha; Hameed, Abdul; Ahmed, Safia (May 2008). "Biological degradation of plastics: A comprehensive review". Biotechnology Advances 26 (3): 246–265. doi:10.1016/j.biotechadv.2007.12.005. PMID 18337047.
38. ↑ Singh, Narinder; Hui, David; Singh, Rupinder; Ahuja, I.P.S.; Feo, Luciano; Fraternali, Fernando (April 2017). "Recycling of plastic solid waste: A state of art review and future applications". Composites Part B: Engineering 115: 409–422. doi:10.1016/j.compositesb.2016.09.013.
39. ↑ Hopewell, Jefferson; Dvorak, Robert; Kosior, Edward (27 July 2009). "Plastics recycling: challenges and opportunities". Philosophical Transactions of the Royal Society B: Biological Sciences 364 (1526): 2115–2126. doi:10.1098/rstb.2008.0311. PMID 19528059.
40. ↑ Yin, Shi; Tuladhar, Rabin; Shi, Feng; Shanks, Robert A.; Combe, Mark; Collister, Tony (December 2015). "Mechanical reprocessing of polyolefin waste: A review". Polymer Engineering & Science 55 (12): 2899–2909. doi:10.1002/pen.24182.
41. ↑ Babetto, Alex S.; Antunes, Marcela C.; Bettini, Sílvia H. P.; Bonse, Baltus C. (February 2020). "A Recycling-Focused Assessment of the Oxidative Thermomechanical Degradation of HDPE Melt Containing Pro-oxidant". Journal of Polymers and the Environment 28 (2): 699–712. doi:10.1007/s10924-019-01641-6. Bibcode: 2020JPEnv..28..699B. https://repositorio.fei.edu.br/handle/FEI/3410.
42. ↑ Aldas, Miguel; Paladines, Andrea; Valle, Vladimir; Pazmiño, Miguel; Quiroz, Francisco (2018). "Effect of the Prodegradant-Additive Plastics Incorporated on the Polyethylene Recycling". International Journal of Polymer Science 2018: 1–10. doi:10.1155/2018/2474176.
43. ↑ Eriksen, M.K.; Christiansen, J.D.; Daugaard, A.E.; Astrup, T.F. (August 2019). "Closing the loop for PET, PE and PP waste from households: Influence of material properties and product design for plastic recycling". Waste Management 96: 75–85. doi:10.1016/j.wasman.2019.07.005. PMID 31376972. Bibcode: 2019WaMan..96...75E. https://backend.orbit.dtu.dk/ws/files/186061805/Eriksen_et_al._2019_ORBIT.pdf.
44. ↑ Kaminsky, W; Predel, M; Sadiki, A (September 2004). "Feedstock recycling of polymers by pyrolysis in a fluidised bed". Polymer Degradation and Stability 85 (3): 1045–1050. doi:10.1016/j.polymdegradstab.2003.05.002.
45. ↑ Kumagai, Shogo; Yoshioka, Toshiaki (1 November 2016). "Feedstock Recycling via Waste Plastic Pyrolysis". Journal of the Japan Petroleum Institute 59 (6): 243–253. doi:10.1627/jpi.59.243. https://www.jstage.jst.go.jp/article/jpi/59/6/59_243/_article/-char/en.
46. ↑ Rahimi, AliReza; García, Jeannette M. (June 2017). "Chemical recycling of waste plastics for new materials production". Nature Reviews Chemistry 1 (6): 0046. doi:10.1038/s41570-017-0046.
47. ↑ Coates, Geoffrey W.; Getzler, Yutan D. Y. L. (July 2020). "Chemical recycling to monomer for an ideal, circular polymer economy". Nature Reviews Materials 5 (7): 501–516. doi:10.1038/s41578-020-0190-4. Bibcode: 2020NatRM...5..501C.
48. ↑ Aguado, J.; Serrano, D. P.; Escola, J. M. (5 November 2008). "Fuels from Waste Plastics by Thermal and Catalytic Processes: A Review". Industrial & Engineering Chemistry Research 47 (21): 7982–7992. doi:10.1021/ie800393w.
49. ↑ Wei, Ren; Zimmermann, Wolfgang (November 2017). "Microbial enzymes for the recycling of recalcitrant petroleum-based plastics: how far are we?". Microbial Biotechnology 10 (6): 1308–1322. doi:10.1111/1751-7915.12710. PMID 28371373.
50. ↑ Geyer, B.; Lorenz, G.; Kandelbauer, A. (2016). "Recycling of poly(ethylene terephthalate) – A review focusing on chemical methods". Express Polymer Letters 10 (7): 559–586. doi:10.3144/expresspolymlett.2016.53.
51. ↑ Ru, Jiakang; Huo, Yixin; Yang, Yu (21 April 2020). "Microbial Degradation and Valorization of Plastic Wastes". Frontiers in Microbiology 11: 442. doi:10.3389/fmicb.2020.00442. PMID 32373075.
52. ↑ Wierckx, Nick; Prieto, M. Auxiliadora; Pomposiello, Pablo; Lorenzo, Victor; O'Connor, Kevin; Blank, Lars M. (November 2015). "Plastic waste as a novel substrate for industrial biotechnology". Microbial Biotechnology 8 (6): 900–903. doi:10.1111/1751-7915.12312. PMID 26482561.
53. ↑ Celina, Mathew C.; Linde, Erik; Martinez, Estevan (March 2021). "Carbonyl Identification and Quantification Uncertainties for Oxidative Polymer Degradation". Polymer Degradation and Stability 188. doi:10.1016/j.polymdegradstab.2021.109550.

* v
* t
* e

Plastics

Chemical types|

* Acrylonitrile butadiene styrene (ABS)
* Cross-linked polyethylene (PEX, XLPE)
* Ethylene vinyl acetate (EVA)
* Poly(methyl methacrylate) (PMMA)
* Poly(ethyl methacrylate) (PEMA)
* Polyacrylic acid (PAA)
* Polyamide (PA)
* Polybutylene (PB)
* Polybutylene terephthalate (PBT)
* Polycarbonate (PC)
* Polyetheretherketone (PEEK)
* Polyester (PEs)
* Polyethylene (PE)
* Polyethylene terephthalate (PET, PETE)
* Polyimide (PI)
* Polylactic acid (PLA)
* Polyoxymethylene (POM)
* Polyphenyl ether (PPE)
* Polypropylene (PP)
* Polystyrene (PS)
* Polysulfone (PES)
* Polytetrafluoroethylene (PTFE)
* Polyurethane (PU)
* Polyvinyl chloride (PVC)
* Polyvinylidene chloride (PVDC)
* Styrene maleic anhydride (SMA)
* Styrene-acrylonitrile (SAN)

Mechanical types|

* Thermoplastic
* Thermosetting polymer
* Duroplast
* Corrugated plastic
* Polymeric foam
* High performance plastics

Additives|

* Polymer additive
* Colorants
* Plasticizer
* Stabilizer for polymers
* Biodegradable additives
* Filler (materials)

Plastics processing|

* injection moulding
* plastics extrusion
* stretch-blow molding
* thermoforming
* compression molding
* calendering
* transfer molding
* laminating
* fiberglass molding
* pultrusion
* filament winding
* vacuum forming
* rotational molding

Products|

* Plastics industry
* Commodity plastics
* Engineering plastics
* High-performance plastics
* Plastic film
* Plastic bottle
* Plastic bag
* Plastic shopping bag
* Plastic cutlery
* Blister pack
* Foam food container
* Construction
* Geosynthetics
* Category:Plastics applications

Environment and health|

* v
* t
* e

Health issues of plastics and polyhalogenated compounds (PHCs)

Plasticizers: Phthalates|

* DIBP
* DBP
* BBP (BBzP)
* DIHP
* DEHP (DOP)
* DIDP
* DINP

Miscellaneous plasticizers|

* Organophosphates
* Adipates (DEHA
* DOA)

Monomers|

* Bisphenol A (BPA, in Polycarbonates)
* Vinyl chloride (in PVC)

Miscellaneous additives incl. PHCs|

* PBDEs
* PCBs
* Organotins
* PFCs
* Perfluorooctanoic acid

Health issues|

* Teratogen
* Carcinogen
* Endocrine disruptor
* Diabetes
* Obesity
* Obesogen
* Polymer fume fever

Pollution|

* Plastic pollution
* Rubber pollution
* Great Pacific garbage patch
* Persistent organic pollutant
* Dioxins
* List of environmental health hazards

Regulations|

* California Proposition 65
* European REACH regulation
* Japan Toxic Substances Law
* Toxic Substances Control Act

Waste|

* Plastic pollution
* Great Pacific garbage patch
* Persistent organic pollutant
* Dioxins
* List of environmental health hazards
* Plastic recycling
* Biodegradable plastic

Identification codes

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Polymer degradation. Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Chemistry:Polymer_degradation&oldid=4340411"
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template